LMucko/crystallography-open-database huggingface dataset:
Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire: Synchrotron X-ray powder diffraction and Rietveld analysis Sample: T = 300 C, phase I
Lee, Y.; Hriljac, J. A.; Vogt, T.; American Mineralogist 90 (2005) 247–251; doi:

data_9016783
_publ_section_title
;
 Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire:
 Synchrotron X-ray powder diffraction and Rietveld analysis
 Sample: T = 300 C, phase I
;
_journal_name_full               'American Mineralogist'
_journal_page_first              247
_journal_page_last               251
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Al2.315 Ca0.474 H4 Na1.462 O12 Si2.685'
_chemical_name_mineral           Gonnardite
_space_group_IT_number           122
_space_group_name_Hall           'I -4 2bw'
_space_group_name_H-M_alt        'I -4 2 d'
_symmetry_space_group_name_H-M   'I -4 2 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.9202
_cell_length_b                   12.9202
_cell_length_c                   6.6950
_cell_volume                     1117.607
_database_code_amcsd             0003725
_diffrn_ambient_temperature      573.15
_exptl_crystal_density_diffrn    2.297
_cod_data_source_file            inputs/fixed/downloads/03/03757.cif
_cod_data_source_block           03757
_cod_original_formula_sum        '(Si2.685 Al2.315) O12 Na1.462 Ca.474 H4'
_cod_database_code               9016783
_cod_duplicate_entry 9003632
Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire: Synchrotron X-ray powder diffraction and Rietveld analysis Sample: T = 300 C, phase II
Lee, Y.; Hriljac, J. A.; Vogt, T.; American Mineralogist 90 (2005) 247–251; doi:

data_9016784
_publ_section_title
;
 Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire:
 Synchrotron X-ray powder diffraction and Rietveld analysis
 Sample: T = 300 C, phase II
;
_journal_name_full               'American Mineralogist'
_journal_page_first              247
_journal_page_last               251
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al2.315 Ca0.474 H0.804 Na1.462 O10.402 Si2.685'
_chemical_name_mineral           Gonnardite
_space_group_IT_number           122
_space_group_name_Hall           'I -4 2bw'
_space_group_name_H-M_alt        'I -4 2 d'
_symmetry_space_group_name_H-M   'I -4 2 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.1503
_cell_length_b                   13.1503
_cell_length_c                   6.2469
_cell_volume                     1080.279
_database_code_amcsd             0003726
_diffrn_ambient_temperature      573.15
_exptl_crystal_density_diffrn    2.199
_cod_data_source_file            inputs/fixed/downloads/03/03758.cif
_cod_data_source_block           03758
_cod_original_formula_sum
'(Si2.685 Al2.315) O10.402 Na1.462 Ca.474 H.804'
_cod_database_code               9016784
_cod_duplicate_entry 9003633
Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire: Synchrotron X-ray powder diffraction and Rietveld analysis Sample: T = 100 C
Lee, Y.; Hriljac, J. A.; Vogt, T.; American Mineralogist 90 (2005) 247–251; doi:

data_9016785
_publ_section_title
;
 Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire:
 Synchrotron X-ray powder diffraction and Rietveld analysis
 Sample: T = 100 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              247
_journal_page_last               251
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Al2.315 Ca0.474 H4.74 Na1.462 O12.37 Si2.685'
_chemical_name_mineral           Tetranatrolite
_space_group_IT_number           122
_space_group_name_Hall           'I -4 2bw'
_space_group_name_H-M_alt        'I -4 2 d'
_symmetry_space_group_name_H-M   'I -4 2 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.0666
_cell_length_b                   13.0666
_cell_length_c                   6.6632
_cell_volume                     1137.648
_database_code_amcsd             0003728
_diffrn_ambient_temperature      373.15
_exptl_crystal_density_diffrn    2.296
_cod_data_source_file            inputs/fixed/downloads/03/03760.cif
_cod_data_source_block           03760
_cod_original_formula_sum        '(Si2.685 Al2.315) O12.37 Na1.462 Ca.474 H4.74'
_cod_database_code               9016785
_cod_duplicate_entry 9003630
Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire: Synchrotron X-ray powder diffraction and Rietveld analysis Sample: T = 200 C
Lee, Y.; Hriljac, J. A.; Vogt, T.; American Mineralogist 90 (2005) 247–251; doi:

data_9016786
_publ_section_title
;
 Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire:
 Synchrotron X-ray powder diffraction and Rietveld analysis
 Sample: T = 200 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              247
_journal_page_last               251
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al2.315 Ca0.474 H4.204 Na1.462 O12.102 Si2.685'
_chemical_name_mineral           Tetranatrolite
_space_group_IT_number           122
_space_group_name_Hall           'I -4 2bw'
_space_group_name_H-M_alt        'I -4 2 d'
_symmetry_space_group_name_H-M   'I -4 2 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.9815
_cell_length_b                   12.9815
_cell_length_c                   6.6808
_cell_volume                     1125.844
_database_code_amcsd             0003729
_diffrn_ambient_temperature      473.15
_exptl_crystal_density_diffrn    2.291
_cod_data_source_file            inputs/fixed/downloads/03/03761.cif
_cod_data_source_block           03761
_cod_original_formula_sum
'(Si2.685 Al2.315) O12.102 Na1.462 Ca.474 H4.204'
_cod_database_code               9016786
_cod_duplicate_entry 9003631
Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire: Synchrotron X-ray powder diffraction and Rietveld analysis Sample: T = 300 C, phase I
Lee, Y.; Hriljac, J. A.; Vogt, T.; American Mineralogist 90 (2005) 247–251; doi:

data_9016787
_publ_section_title
;
 Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire:
 Synchrotron X-ray powder diffraction and Rietveld analysis
 Sample: T = 300 C, phase I
;
_journal_name_full               'American Mineralogist'
_journal_page_first              247
_journal_page_last               251
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Al2.315 Ca0.474 H4 Na1.462 O12 Si2.685'
_chemical_name_mineral           Tetranatrolite
_space_group_IT_number           122
_space_group_name_Hall           'I -4 2bw'
_space_group_name_H-M_alt        'I -4 2 d'
_symmetry_space_group_name_H-M   'I -4 2 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.9202
_cell_length_b                   12.9202
_cell_length_c                   6.6950
_cell_volume                     1117.607
_database_code_amcsd             0003730
_diffrn_ambient_temperature      573.15
_exptl_crystal_density_diffrn    2.297
_cod_data_source_file            inputs/fixed/downloads/03/03762.cif
_cod_data_source_block           03762
_cod_original_formula_sum        '(Si2.685 Al2.315) O12 Na1.462 Ca.474 H4'
_cod_database_code               9016787
_cod_duplicate_entry 9003632
Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire: Synchrotron X-ray powder diffraction and Rietveld analysis Sample: T = 300 C, phase II
Lee, Y.; Hriljac, J. A.; Vogt, T.; American Mineralogist 90 (2005) 247–251; doi:

data_9016788
_publ_section_title
;
 Variable-temperature structural studies of tetranatrolite from Mt. Saint-Hilaire:
 Synchrotron X-ray powder diffraction and Rietveld analysis
 Sample: T = 300 C, phase II
;
_journal_name_full               'American Mineralogist'
_journal_page_first              247
_journal_page_last               251
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al2.315 Ca0.474 H0.804 Na1.462 O10.402 Si2.685'
_chemical_name_mineral           Tetranatrolite
_space_group_IT_number           122
_space_group_name_Hall           'I -4 2bw'
_space_group_name_H-M_alt        'I -4 2 d'
_symmetry_space_group_name_H-M   'I -4 2 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.1503
_cell_length_b                   13.1503
_cell_length_c                   6.2469
_cell_volume                     1080.279
_database_code_amcsd             0003731
_diffrn_ambient_temperature      573.15
_exptl_crystal_density_diffrn    2.199
_cod_data_source_file            inputs/fixed/downloads/03/03763.cif
_cod_data_source_block           03763
_cod_original_formula_sum
'(Si2.685 Al2.315) O10.402 Na1.462 Ca.474 H.804'
_cod_database_code               9016788
_cod_duplicate_entry 9003633
The crystal-chemistry of holmquistites: Ferroholmquistite from Greenbushes (Western Australia) and hints for compositional constraints in B-Li amphiboles Sample: HS 119915 Siberia
Camara, F.; Oberti, R.; American Mineralogist 90 (2005) 1167–1176; doi:

data_9016789
_publ_section_title
;
 The crystal-chemistry of holmquistites: Ferroholmquistite from
 Greenbushes (Western Australia) and
 hints for compositional constraints in B-Li amphiboles
 Sample: HS 119915 Siberia
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1167
_journal_page_last               1176
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al1.97 F0.03 Fe1.23 H3.94 Li1.98 Mg1.8 Mn0.02 Na0.03 O23.97 Si7.99 Zn0.01'
_chemical_name_mineral           Holmquistite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   18.277
_cell_length_b                   17.650
_cell_length_c                   5.2736
_cell_volume                     1701.206
_database_code_amcsd             0003813
_exptl_crystal_density_diffrn    3.101
_cod_data_source_file            inputs/fixed/downloads/03/03844.cif
_cod_data_source_block           03844
_cod_original_formula_sum
'Mg1.8 Fe1.23 Mn.02 Al1.97 Zn.01 Li1.98 Na.03 Si7.99 O23.97 F.03 H3.94'
_cod_database_code               9016789
The crystal-chemistry of holmquistites: Ferroholmquistite from Greenbushes (Western Australia) and hints for compositional constraints in B-Li amphiboles Sample: Siberia
Camara, F.; Oberti, R.; American Mineralogist 90 (2005) 1167–1176; doi:

data_9016790
_publ_section_title
;
 The crystal-chemistry of holmquistites: Ferroholmquistite from
 Greenbushes (Western Australia) and
 hints for compositional constraints in B-Li amphiboles
 Sample: Siberia
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1167
_journal_page_last               1176
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al1.98 F0.02 Fe1.2 H3.96 Li1.71 Mg1.89 Mn0.01 Na0.03 O24 Si7.98'
_chemical_name_mineral           Holmquistite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   18.277
_cell_length_b                   17.646
_cell_length_c                   5.2792
_cell_volume                     1702.626
_database_code_amcsd             0003814
_exptl_crystal_density_diffrn    3.088
_cod_data_source_file            inputs/fixed/downloads/03/03845.cif
_cod_data_source_block           03845
_cod_original_formula_sum
'Mg1.89 Fe1.2 Mn.01 Al1.98 Li1.71 Na.03 Si7.98 O24 F.02 H3.96'
_cod_database_code               9016790
The crystal-chemistry of holmquistites: Ferroholmquistite from Greenbushes (Western Australia) and hints for compositional constraints in B-Li amphiboles Sample: Rwanda
Camara, F.; Oberti, R.; American Mineralogist 90 (2005) 1167–1176; doi:

data_9016791
_publ_section_title
;
 The crystal-chemistry of holmquistites: Ferroholmquistite from
 Greenbushes (Western Australia) and
 hints for compositional constraints in B-Li amphiboles
 Sample: Rwanda
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1167
_journal_page_last               1176
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al1.76 F0.07 Fe1.2 H3.86 Li1.97 Mg2.01 Mn0.04 Na0.02 O23.93 Si8 Zn0.01'
_chemical_name_mineral           Holmquistite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   18.2754
_cell_length_b                   17.6569
_cell_length_c                   5.2738
_cell_volume                     1701.786
_database_code_amcsd             0003815
_exptl_crystal_density_diffrn    3.096
_cod_data_source_file            inputs/fixed/downloads/03/03846.cif
_cod_data_source_block           03846
_cod_original_formula_sum
'Mg2.01 Fe1.2 Mn.04 Al1.76 Zn.01 Li1.97 Na.02 Si8 O23.93 F.07 H3.86'
_cod_database_code               9016791
The crystal-chemistry of holmquistites: Ferroholmquistite from Greenbushes (Western Australia) and hints for compositional constraints in B-Li amphiboles Sample: Zaire
Camara, F.; Oberti, R.; American Mineralogist 90 (2005) 1167–1176; doi:

data_9016792
_publ_section_title
;
 The crystal-chemistry of holmquistites: Ferroholmquistite from
 Greenbushes (Western Australia) and
 hints for compositional constraints in B-Li amphiboles
 Sample: Zaire
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1167
_journal_page_last               1176
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al1.34 F0.09 Fe1.26 H3.82 Li1.98 Mg2.35 Mn0.04 Na0.05 O23.91 Si8 Zn0.01'
_chemical_name_mineral           Holmquistite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   18.3345
_cell_length_b                   17.6955
_cell_length_c                   5.2764
_cell_volume                     1711.865
_database_code_amcsd             0003816
_exptl_crystal_density_diffrn    3.081
_cod_data_source_file            inputs/fixed/downloads/03/03847.cif
_cod_data_source_block           03847
_cod_original_formula_sum
'Mg2.35 Fe1.26 Mn.04 Zn.01 Al1.34 Li1.98 Na.05 Si8 O23.91 F.09 H3.82'
_cod_database_code               9016792
The crystal-chemistry of holmquistites: Ferroholmquistite from Greenbushes (Western Australia) and hints for compositional constraints in B-Li amphiboles Sample: Uto, Sweden
Camara, F.; Oberti, R.; American Mineralogist 90 (2005) 1167–1176; doi:

data_9016793
_publ_section_title
;
 The crystal-chemistry of holmquistites: Ferroholmquistite from
 Greenbushes (Western Australia) and
 hints for compositional constraints in B-Li amphiboles
 Sample: Uto, Sweden
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1167
_journal_page_last               1176
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al1.3 F0.13 Fe1.3 H3.74 Li1.93 Mg2.32 Mn0.06 Na0.1 O23.87 Si8 Zn0.01'
_chemical_name_mineral           Holmquistite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   18.335
_cell_length_b                   17.693
_cell_length_c                   5.2743
_cell_volume                     1710.989
_database_code_amcsd             0003817
_exptl_crystal_density_diffrn    3.092
_cod_data_source_file            inputs/fixed/downloads/03/03848.cif
_cod_data_source_block           03848
_cod_original_formula_sum
'Mg2.32 Fe1.3 Mn.06 Al1.3 Zn.01 Li1.93 Na.1 Si8 O23.87 F.13 H3.74'
_cod_database_code               9016793
The crystal-chemistry of holmquistites: Ferroholmquistite from Greenbushes (Western Australia) and hints for compositional constraints in B-Li amphiboles Sample: Norway
Camara, F.; Oberti, R.; American Mineralogist 90 (2005) 1167–1176; doi:

data_9016794
_publ_section_title
;
 The crystal-chemistry of holmquistites: Ferroholmquistite from
 Greenbushes (Western Australia) and
 hints for compositional constraints in B-Li amphiboles
 Sample: Norway
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1167
_journal_page_last               1176
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al1.33 F0.1 Fe1.26 H3.8 Li1.93 Mg2.42 Mn0.04 Na0.05 O23.9 Si8 Zn0.01'
_chemical_name_mineral           Holmquistite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   18.336
_cell_length_b                   17.693
_cell_length_c                   5.2755
_cell_volume                     1711.472
_database_code_amcsd             0003818
_exptl_crystal_density_diffrn    3.086
_cod_data_source_file            inputs/fixed/downloads/03/03849.cif
_cod_data_source_block           03849
_cod_original_formula_sum
'Mg2.42 Fe1.26 Mn.04 Al1.33 Zn.01 Li1.93 Na.05 Si8 O23.9 F.1 H3.8'
_cod_database_code               9016794
The crystal-chemistry of holmquistites: Ferroholmquistite from Greenbushes (Western Australia) and hints for compositional constraints in B-Li amphiboles Sample: Greenbushes, W Australia
Camara, F.; Oberti, R.; American Mineralogist 90 (2005) 1167–1176; doi:

data_9016795
_publ_section_title
;
 The crystal-chemistry of holmquistites: Ferroholmquistite from
 Greenbushes (Western Australia) and
 hints for compositional constraints in B-Li amphiboles
 Sample: Greenbushes, W Australia
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1167
_journal_page_last               1176
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum
'Al1.89 F0.03 Fe1.71 H3.94 K0.01 Li1.88 Mg1.47 Mn0.01 Na0.04 O23.97 Si8'
_chemical_name_mineral           Ferro-holmquistite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   18.2872
_cell_length_b                   17.6797
_cell_length_c                   5.2784
_cell_volume                     1706.571
_database_code_amcsd             0003812
_exptl_crystal_density_diffrn    3.152
_cod_data_source_file            inputs/fixed/downloads/03/03850.cif
_cod_data_source_block           03850
_cod_original_formula_sum
'Mg1.47 Fe1.71 Mn.01 Al1.89 Li1.88 Na.04 K.01 Si8 O23.97 F.03 H3.94'
_cod_database_code               9016795
Sideronatrite, Na2Fe(SO4)2(OH)*3H2O: Crystal structure of the orthorhombic polytype and OD character analysis
Scordari, F.; Ventruti, G.; American Mineralogist 94 (2009) 1679–1686; doi:

data_9016796
_publ_section_title
;
 Sideronatrite, Na2Fe(SO4)2(OH)*3H2O: Crystal structure of
 the orthorhombic polytype and OD character analysis
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1679
_journal_page_last               1686
_journal_volume                  94
_journal_year                    2009
_chemical_compound_source        'Sierra Gorda, Chile'
_chemical_formula_sum            'Fe H7 Na2 O12 S2'
_chemical_name_mineral           Sideronatrite
_space_group_IT_number           19
_space_group_name_Hall           'P 2ac 2ab'
_space_group_name_H-M_alt        'P 21 21 21'
_symmetry_space_group_name_H-M   'P 21 21 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.265
_cell_length_b                   20.522
_cell_length_c                   7.120
_cell_volume                     1061.537
_database_code_amcsd             0020665
_exptl_crystal_density_diffrn    2.284
_cod_data_source_file            inputs/fixed/downloads/04/04994.cif
_cod_data_source_block           04994
_cod_original_formula_sum        'Na2 Fe S2 O12 H7'
_cod_database_code               9016796
Semi-ordered crystalline structure of the Santa Olalla vermiculite inferred from X-ray powder diffraction
Arguelles, A.; Leoni, M.; Blanco, J. A.; Marcos, C.; American Mineralogist 95 (2010) 126–134; doi:

data_9016797
_publ_section_title
;
 Semi-ordered crystalline structure of the Santa Olalla vermiculite
 inferred from X-ray powder diffraction
;
_journal_name_full               'American Mineralogist'
_journal_page_first              126
_journal_page_last               134
_journal_volume                  95
_journal_year                    2010
_chemical_compound_source        'Santa Olalla, Toledo Province, Spain'
_chemical_formula_sum
'Al2.936 Ca0.06 Fe0.438 H17.6 Mg5.68 Na0.04 O30.8 Si5.664 Ti0.042'
_chemical_name_mineral           Vermiculite
_space_group_IT_number           1
_space_group_name_Hall           'P 1'
_space_group_name_H-M_alt        'P 1'
_symmetry_space_group_name_H-M   'P 1'
_cell_angle_alpha                90.0002
_cell_angle_beta                 97.0909
_cell_angle_gamma                90.0002
_cell_formula_units_Z            1
_cell_length_a                   5.3434
_cell_length_b                   9.254
_cell_length_c                   14.34
_cell_volume                     703.658
_database_code_amcsd             0020497
_exptl_crystal_density_diffrn    2.163
_cod_data_source_file            inputs/fixed/downloads/04/04995.cif
_cod_data_source_block           04995
_cod_original_formula_sum
'Mg5.68 Fe.438 Al2.936 Ti.042 Ca.06 Na.04 Si5.664 O30.8 H17.6'
_cod_database_code               9016797